High‐Areal‐Capacity Silicon Electrodes with Low‐Cost Silicon ... ......
Embed Size (px)
Transcript of High‐Areal‐Capacity Silicon Electrodes with Low‐Cost Silicon ... ......
IC A TIO
© 2015 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim (1 of 8) 1401826wileyonlinelibrary.com
High-Areal-Capacity Silicon Electrodes with Low-Cost Silicon Particles Based on Spatial Control of Self-Healing Binder
Zheng Chen , Chao Wang , Jeffrey Lopez , Zhenda Lu , Yi Cui ,* and Zhenan Bao*
Dr. Z. Chen, Dr. C. Wang, J. Lopez, Prof. Z. Bao Department of Chemical Engineering Stanford University Stanford , CA 94305 , USA E-mail: email@example.com Dr. Z. Lu, Prof. Y. Cui Department of Materials Science and Engineering Stanford University Stanford , CA 94305 , USA E-mail: firstname.lastname@example.org Prof. Y. Cui Stanford Institute for Materials and Energy Sciences SLAC National Accelerator Laboratory Menlo Park , CA 94205 , USA
energy density based on the whole cell. Currently, only a few reported Si nanostructures can reach an areal capacity of >3 mAh cm −2 . [ 12,27 ]
Recently, we reported the use of self-healing polymers (SHPs) to stabilize low-cost Si microparticle (SiMP) anodes. SHPs have both mechanical and electrical healing capabili- ties, which allow cracks and damages to the conduction paths to repeatedly heal during battery cycling. SiMP electrodes with 90 cycles and capacity loading of ≈1 mAh cm −2 and 45 cycles with areal capacity loading of 1.9 mAh cm −2 were reported. [ 42 ] However, long-term cycling stability and high Si mass loading have not yet been achieved. Similarly, a binder incorporating Meldrum’s acid showed some self-healing effect that can improve the cycling performance of Si electrodes. Yet such elec- trodes were still based on costly Si nanoparticles (
IC A TI
© 2015 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim1401826 (2 of 8) wileyonlinelibrary.com
Accordingly, it is essential to build a robust interface between Si particles and the SHP to maintain electrode integrity. At the electrode level, the electrical connection between particles can be damaged by the large volume change of Si lithiation/del- ithiation, resulting in capacity decay. At the individual particle level, crack formation can cause the loss of electrical contact and detachment of active materials. In our previous study, we coated SHP only on top of the Si particle electrodes, at a thick- ness of 200 nm–3 µm. [ 42 ] Therefore, a signifi cant fraction of Si material was not in close proximity to the SHP. In our new electrode design described herein, we have intentionally distrib- uted the SHP 3D into the Si particle layer, in order to provide a faster healing response owing to the shorter diffusion lengths of SHP to the generated fracture sites.
Figure 1 a–c shows the schematic of the 3D design com- pared with top layer coating. Si electrodes were fabricated by coating a Si particle slurry on Cu substrates, followed by drying and calendaring (Figure 1 a). SHP/CB polymer composite was then coated on the Si electrode using a blade to form the top layer (Figure 1 b). Repeatedly blading under heating condition (120≈150 °C), is crucial to allow the SHP/CB to infi ltrate into the entire thickness of the Si layer, forming a 3D distribution of SHP/CB inside the Si electrode (Si-SHP/CB, Figure 1 c). The bulk density of Si fi lm was calculated to be 1.0–1.1 g cm −3 for particles with ≈800-nm diameter, corresponding to a porosity of ≈60% (Figure 1 d). After coating the SHP/CB on the top layer of Si fi lm, without heating, a clear boundary between Si and Si-SHP/CB can be observed from the cross-section view of the electrodes (Figure 1 e). After repeated coating under heating, a 3D spatial distribution of SHP/CB can be clearly seen inside the whole Si electrode (Figure 1 f).
Since the healing of fractures relies on interactions between SHP and Si particles, we hypothesize that particle sizes may infl uence the healing behavior. For large SiMPs (e.g., a few microns), a full lithiation/delithiation not only produces large cracks, but also induces pulverization with a large number of small cracks between fragments. To maintain electrode activity, conductive pathways need to be rebuilt through
diffusion of SHP into these cracks. This requires a contin- uous healing pathway, and is especially diffi cult. As a result, capacity loss occurs due to increased dead zones where elec- tron and ion transport are interrupted. In contrast, smaller Si particles have higher surface areas and more binding sites with SHP. They are also subjected to less pulverization. Even if fractures were to occur, the diffusion of SHP and healing of small cracks can proceed more effi ciently due to a shorter dif- fusion length. In the extreme case of ultrasmall SiNPs (e.g., 300% stretchability).
To verify the above hypothesis, Si-SHP/CB electrodes were fabricated using Si particles with different sizes that range in between 250 nm and 3.5 µm (see ‘‘Experimental Section”). They were obtained by a simple yet effective solution precipitation– fl oatation selection process (Figure S2, Supporting Informa- tion). As shown in Figure 2 , different electrodes showed quite different cycling performances. For 3.5 µm SiMPs (Figure 2 a), most of the Si electrode consists of large particles and the elec- trodes showed a low-initial delithiation capacity (≈1100 mAh g −1 at C/20), which may be due to slow lithium-ion diffusion and high lithiation overpotential caused by activation energy barrier of large particles. [ 4,5,47 ] The rapid capacity decrease upon cycling is attributed to the insuffi cient healing capability of the SHP binder for very large Si particles as discussed above. 1-µm SiMP electrodes (Figure S3, Supporting Information) showed a much higher initial delithiation capacity of 2510 mAh g –1 . In this case, although more than 50% of particles are ≈1 µm (Figure S3b, Supporting Information), a small number of larger particles (2–6 µm) contributed to >80% of the total volume (Figure S3c, Supporting Information). Although gradual capacity decay was still observed, the capacity retention was clearly improved, as ≈70% of capacity was retained even after about 100 cycles (Figure S3d, Supporting Information). The increased cycling stability was ascribed to the enhanced healing capability from a better Si-SHP interface. As the particle size is reduced to around 800 nm (Figure 2 b), the electrodes are able to deliver
Adv. Energy Mater. 2015, 1401826
Figure 1. Electrode design toward tuning spatial distribution of SHP/CB in Si layer. a–c) Schematic design of Si-SHP/CB electrodes. d–f) SEM images of Si and Si-SHP/CB electrodes. d) Pure Si electrodes made from Si particles. e) SHP/CB layer coated on top of Si electrodes with one-time blading. f) Si electrodes fi lled with SHP/CB forming a 3D distribution inside electrodes from repeated blading under heating.
IC A TIO
© 2015 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim (3 of 8) 1401826wileyonlinelibrary.com
an even higher initial delithiation capacity of 2620 mAh g −1 (corresponding to an areal capacity of 1.3 mAh cm −2 ) due to the faster lithium reaction kinetics. While ≈95% of whole Si volume is from particles with diameter of 800 nm or larger, the elec- trodes maintained an impressive ≈80% of their initial capacity after 500 cycles. This comparative study confi rms that carefully
reduced Si particle size contributes to enhanced Si-SHP inter- face and better electrode structure.
As expected, further decreasing the Si particle size provides an even better cycling stability. For 500- and 250-nm Si particles (Fig- ures S4 and S5, Supporting Information), their initial delithiation capacity was ≈2600 and 2200 mAh g −1 , and the electrode capacity
Adv. Energy Mater. 2015, 1401826
Figure 2. Effect of Si particle size on electrode cycling performance. a–c) SEM images (left) of Si particles, corresponding particle size distributions (middle) and volume fraction of each particle size (right) obtained from the precipitation–fl oatation-based selection process. d) Cycling stability of different Si-SHP/CB electrodes (a, b, and c correspond to Si particles shown above) with Si mass loading of 0.5–0.6 mg cm −2 .
IC A TI
© 2015 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim1401826 (4 of 8) wileyonlinelibrary.com
retention was ≈80% after 550 and 600 cycles, respectively. Even though the particle size decreased dramatically, the fi rst-cycle CE remained similar (86%–88%) (Figure S6, Supporting Informa- tion), which are much higher than common nanostructured or nanoporous Si electrodes. [ 11,12,15,27,48 ] For 30-nm SiNPs (Figure 2 c), the electrodes showed no obvious capacity decay even after 1000 cycles (Figure S7, Supporting Information), regardless of the relatively low fi rst-cycle CE (73%). Note that the relatively low capacity of SiNPs-based electrodes may be due to their large electrode series resistance (ESR) (Figures S7 and S8, Supporting Information) resulted from the oxide layer on the SiNPs surface and relatively small pore size in the electrodes. Such a stable cycling performance is comparable to the most effective nano- structured Si electrodes while our electrode here has